Download presentation

Presentation is loading. Please wait.

Published byRaymond Bridgett Modified over 3 years ago

1
Tuning eigenstate-energies of InGaAs Quantum-Dots using lateral electric fields W. Prestel, H. Krenner, J. J. Finley St. Petersburg – JASS 2004

2
Outline Introduction –Growth of self-assembled Quantum Dots (SAQDs) –electric fields on QDs Work in progress: single QDs in lateral electric fields Benefit of lateral electric fields –structural information about QDs –Implementation of CNOT Gate

3
Self-Assembly of Quantum Dots Stranski-Krastanov Frank-van der Merwe Volmer-Weber used for usual heterostructures: unstrained material systems i.e. GaAs/AlAs similar to rain drops on window strained material systems i.e. In(Ga)As/GaAs particular growth conditions i.e. temperature, In content, growth rate formation of pseudomorpic layer: Wetting Layer (WL) growth of islands: strain relaxes in islands

4
In(Ga)As Quantum Dots Lattice constant: –GaAs: 0.57nm –InAs: 0.61nm Lattice mismatch ε = 7% typical surface densities: 0 - 1.000 µm -2

5
Growth on unrotated substrate In Ga constant In:Ga ratio gradually changing In:Ga ratio

6
further processing Overgrowth for optical application Intermixing of materials no surface states low band-gap material surrounded by high band- gap matrix material »0-dimensional confinement occurs naturally can also be driven by thermal annealing »change of confinement potential

7
Quantum Dots – artificial atoms Band Gap (300K) –E g,GaAs = 1.411eV –E g,InAs = 0.356eV » ΔE g up to ~ 1eV "real atom" single QD: "artificial atom"

8
SAQDs – confinement for excitons »optically active exciton (X) states are bound E x,y X z »shell structure »parabolic potential »few particle interaction n = 1 n = 2 n = 1 n = 2

9
growth direction 10nm Electric fields on QDs QCSE: Quantum Confined Stark Effect vertical ( ) fields: well investigated intrinsic dipole p 0 weak polarizability c lateral ( ) fields: not investigated in detail intrinsic dipole p = 0 expected high polarizability c further investigation p intrinsic dipole c polarizability

10
growth direction 10nm Electric fields on QDs QCSE: Quantum Confined Stark Effect p intrinsic dipole c polarizability F ΔE(F) F lateral F vertical ???

11
Work in progress Sample Design –model calculations –strength of electrical field Setup + crash course in PL & PC Characterization of sample

12
Sample Design Substrate: –In 0.5 Ga 0.5 As – QDs in GaAs –surface density: ~ 1.000 QDs/µm 2 –undoped substrate Contact-Design –split-gates –standard optical lithography –contacts-on-top design (2µm gap) 2µm

13
First Approach put QDs in Capacitor 1. order approximation: homogeneous lateral field realisation of metal- semiconductor junction (pinning) »expected field: d U

14
Stability Problems structure died during measurement

15
Model calculations on different Designs GaAs Vacuum GaAs Vacuum GaAs Vacuum

16
Model calculations on different Designs E lateral E vertical

17
Model calculations – contacts on top decreasing d increases field considering homogeneity »trade-off: d = 2µm extraction of geometry factor »f midgap 0.75

18
temperature dependent IV-Curves max. fields: 80-130 kV/cm Dark current measurement

19
µPL/µPC - Setup Spatial Resolution (1µm Spot) Bias dependent optical spectroscopy (PL and PC) Temperature: down to 4.2K U

20
Crash course PL & PC WL Ensemble of QDs single QD

21
Bias dependent PL-Spectra HeNe-excitation (632.8nm) PL disappears @ 13 kV/cm (3.5V)

22
Bias dependent PL & PC HeNe excitation (632.8nm)

23
PC resonant excitation

24
»4-terminal-µCapacitor –different crystal directions –top and back contacts foreseen Sample Design – future plans top view

25
Application 1)Investigation of shape and alloy profile of buried Dots 2)Goal in further future: Implementation of CNOT gate

26
Shape and alloy profile of QDs no non-invasive characterization of overgrown QDs possible structural properties determine electro-optical properties

27
Definition of Qubits QM implementation of CNOT -1-Qbit-System: X 0 in QD | 1 0 empty QD | 0 -2-Qbit-System: Quantum Dot Molecule (QDM): empty dots | 00 ; X 0 in lower dot | 10 ; … | 01 ; … | 11 -coupling of X 0 in QDM via dipole-dipole interaction: Applying lateral field means control of ΔE 10nm E |11 = E |01 + E |10 + ΔE

28
CNOT Gate 1 1 0 0 00 --> 00 01 --> 01 10 --> 11 11 --> 10 0 1 0 on off control bit switches NOT-operation on target bit control bit unaffected by CNOT target bit changed if control bit is 1 initializationapplying gate operationreadout on off target bit consideration purely classical and logic so far: quantum mechanical implementation

29
Implementation PC-Meas control of dot occupation Rabi-oscillation different X 0 -GS-energies a a b ba ab b The above term scheme can be taylored for our needs by applying vertical & lateral fields!!! initializationapplying gate operationreadout

30
Rabi Oscillation

Similar presentations

OK

Observation of Excited Biexciton States in CuCl Quantum Dots : Control of the Quantum Dot Energy by a Photon Itoh Lab. Hiroaki SAWADA Michio IKEZAWA and.

Observation of Excited Biexciton States in CuCl Quantum Dots : Control of the Quantum Dot Energy by a Photon Itoh Lab. Hiroaki SAWADA Michio IKEZAWA and.

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google

Ppt on limitation act malaysia Mba ppt on introduction to business finance Ppt on terrorism in india free download Ppt on natural resources land soil and water Ppt on conservation of momentum Ppt on natural resources and conservation major Animated ppt on magnetism worksheets Ppt on information technology act Ppt on covalent bonding animation Ppt on latest advancement in technology